Photoluminescence of Sn2±-I−-mixed molecular perovskites
Fan, Guang-Meng; Shi, Chao; Qiao, Liang; Li, Hao-Jie; Ye, Heng-Yun; Journal of Materials Chemistry C 6 (2018) 8349–; doi:10.1039/C8TC02587H

data_7237398
_publ_section_title
;
 Photoluminescence of Sn2+--I&#x2212;-mixed molecular perovskites
;
_journal_issue                   31
_journal_name_full               'Journal of Materials Chemistry C'
_journal_page_first              8349
_journal_paper_doi               10.1039/C8TC02587H
_journal_volume                  6
_journal_year                    2018
_chemical_formula_sum            'C7 H20 B3 F12 N3'
_chemical_formula_weight         406.69
_space_group_crystal_system      trigonal
_space_group_IT_number           167
_space_group_name_Hall           '-R 3 2"c'
_space_group_name_H-M_alt        'R -3 c :H'
_atom_sites_solution_hydrogens   mixed
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2018-05-17 deposited with the CCDC.
2018-07-20 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            12
_cell_length_a                   10.213(2)
_cell_length_b                   10.213(2)
_cell_length_c                   53.387(9)
_cell_measurement_reflns_used    3115
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.4546
_cell_measurement_theta_min      2.7621
_cell_volume                     4822.5(16)
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.984
_diffrn_measured_fraction_theta_max 0.983
_diffrn_measurement_device_type  'Rigaku saturn 724'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0572
_diffrn_reflns_av_unetI/netI     0.0479
_diffrn_reflns_Laue_measured_fraction_full 0.984
_diffrn_reflns_Laue_measured_fraction_max 0.983
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       68
_diffrn_reflns_limit_l_min       -58
_diffrn_reflns_number            6151
_diffrn_reflns_point_group_measured_fraction_full 0.984
_diffrn_reflns_point_group_measured_fraction_max 0.983
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.461
_diffrn_reflns_theta_min         3.825
_exptl_absorpt_coefficient_mu    0.196
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.8777
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.680
_exptl_crystal_description       block
_exptl_crystal_F_000             2472
_exptl_crystal_size_max          0.27
_exptl_crystal_size_mid          0.22
_exptl_crystal_size_min          0.18
_refine_diff_density_max         0.514
_refine_diff_density_min         -0.480
_refine_diff_density_rms         0.085
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.129
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     87
_refine_ls_number_reflns         1216
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.129
_refine_ls_R_factor_all          0.1470
_refine_ls_R_factor_gt           0.1254
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1554P)^2^+30.7018P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.3255
_refine_ls_wR_factor_ref         0.3425
_reflns_Friedel_coverage         0.000
_reflns_number_gt                948
_reflns_number_total             1216
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c8tc02587h2.cif
_cod_data_source_block           3
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_exptl_absorpt_correction_type' value 'Multi-scan' was
changed to 'multi-scan' in accordance with the
/home/saulius/struct/COD-crude-data/automatic-downloads/DataCite-retrospective/RSC/depositions/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

Automatic conversion script
Id: cif_fix_values 6909 2019-04-08 15:41:33Z antanas 
;
_cod_original_cell_volume        4823(2)
_cod_database_code               7237398
_shelx_shelxl_version_number     2014/7
_shelx_res_checksum              28570